NO Adsorption on Copper Phthalocyanine Functionalized Graphite † ‡ § ‡ Jun Hong Park, , Pabitra Choudhury, and Andrew C. Kummel*, † ‡ Materials Science & Engineering Program and Departments of Chemistry & Biochemistry, University of California, San Diego and La Jolla, California 92093, United States § Department of Chemical Engineering, New Mexico Tech, Socorro, New Mexico 87801, United States
*S Supporting Information
ABSTRACT: NO dosed on a CuPc monolayer deposited on Au(111) and HOPG is observed by scanning tunneling microscopy. After dosing NO with a supersonic molecular beam source onto CuPc/Au(111), about 7% of CuPc molecules form chemisorbates with NO. Conversely, after dosing onto CuPc/HOPG, only about 0.1% CuPc molecules form chemisorbates with NO, even though the reaction sites appear nearly identical. DFT calculations were employed to elucidate the mechanism which causes the >10× diﬀerence in saturation coverage between NO/CuPc/Au(111) and NO/ CuPc/HOPG. DFT calculations show NO chemisorption with CuPc/Au(111) induces only negligible perturbation in the density of states (DOS) in Au(111) due to large density of states on Au. Conversely, for NO/CuPc/HOPG, there is a large decrease of DOS in graphene around 1 eV due to NO chemisorption on CuPc/graphene consistent with negative charge transfer from graphene to NO. This DOS perturbation of graphene results in decreased binding energy of NO chemisorption in secondary NO sites, consistent with low saturation coverage. The results suggest that although the saturation coverage of NO chemisorbates is low on CuPc/graphene, the DOS of graphene can be altered by low coverages of adsorbates even onto weakly interacting molecules which chemically functionalize the graphene surface.
■ INTRODUCTION structure at high temperature and only a few acids are able to π Graphene, a 2D semiconductor material, consists of sp2 bonded decompose MPcs. MPc molecules have delocalized -electrons, carbon atoms in a honeycomb lattice forming a single layer.1 enabling them to act as electron donors, thereby providing a low activation energy for formation of charge transfer Graphene has high carrier mobility as well as a chemically and 17,28,29 electronically passivated surface, thereby rendering graphene to complexes with oxidizing analytes in chemical sensing. − be a promising electronic material for novel devices.2 5 MPc detection of chemical analytes is induced primarily by Graphene also has potential for chemical sensing platforms, charge transfer reactions between the central metal ion and 6,7 analytes; therefore, in a simpliﬁed model, the analytes act as due to its atomically thin body. The atomically thin body of “ ” 30,31 ﬁ ﬁ graphene allows each carbon atom to directly interact with MPc dopants : Pure MPcs lms of organic thin lm ambient analytes, thereby increasing chemical sensitivity. transistor (OTFT) in vacuum have a Fermi level in the middle of the band gap. However, when MPcs ﬁlms are exposed to However, the surface of graphene is chemically inert, thereby 17,30−32 requiring modiﬁcation for use in electronic and sensor oxidative agents, MPc become p-type semiconductors. − ﬁ devices.8 10 One common approach is oxidation of graphene The induced p-type conductivity of MPc lms has been with chemical reduction, but this oxidation also involves modeled as formation of charge transfer complexes on the 11−13 ﬀ metal centers with oxidative analytes. Oxidative analytes (such introduction of defects. An e ective strategy to modify the 20,31 chemical sensitivity of graphene is functionalization with other as O2), which are electron acceptors, chemisorb on MPc molecules, forming superoxide adducts consisting of oxidized materials without perturbing the graphene electronic structure. + 2− For example, a self-assembly layer by organic molecules can be MPc and O species. During this reaction, electrons are eﬀective for fabrication of graphene based chemical or bio transferred from MPc to analytes. Simultaneously, holes are 14−16 injected into the MPc molecules to form positively charged sensors. + Metal phthalocyanines (MPc) may enhance the sensing MPc . The injection of these holes moves the HOMO edge ﬁ 17 performance of graphene chemical sensors via functionalization. toward the Fermi level forming a p-type MPc lm. Due to − MPc have been widely studied as chemical sensors.17 22 The MPc ﬁlms can be deposited to form well-ordered layers on Received: January 8, 2014 inorganic substrates, including graphene or graphite surfa- Revised: April 19, 2014 − ces.23 27 Moreover, MPcs can maintain their molecular Published: April 22, 2014
© 2014 American Chemical Society 10076 dx.doi.org/10.1021/jp5002258 | J. Phys. Chem. C 2014, 118, 10076−10082 The Journal of Physical Chemistry C Article
Figure 1. Submolecular resolution empty state STM images of a CuPc monolayer surface dosed with NO on Au(111) and HOPG at 150 K. Diluted s NO was dosed by MBS, and nozzle was held at 300 K. Empty state STM images were recorded with V = +2.0 V, It = 20 pA. The pulsing of the MBS was 30 Hz with 100 μs opening time. Scale bars indicate 2 nm. The reacted sites are denoted by circles. (a) Submolecular resolution of CuPc chemisorbed with single NO molecule on Au(111). The center of CuPc is modiﬁed into bright spot. (b) Submolecular resolution of CuPc chemisorbed with single NO molecule on HOPG. The center of CuPc is modiﬁed into bright spot. (c) Chemisorption model of NO with CuPc.
Figure 2. Scanning tunneling spectroscopy (STS) dI/dV curves of unreacted and reacted CuPc molecules. All spectra recorded at the center of the CuPc and were swept from −2 to 2 V. (a) STS dI/dV spectra of NO/CuPc/Au(111). (b) STS dI/dV spectra of NO/CuPc/HOPG. The black spectra indicate STS from unreacted CuPc molecules, while red spectra show STS from CuPc molecules with chemisorbed NO. After NO chemisorption on CuPc molecules, the EF was shifted toward the VB (HOMO) in both NO/CuPc/Au(111) and NO/CuPc/HOPG. these properties and MPc adsorption on graphene not obtained in STM imaging. The Highly Ordered Pyrolytic perturbing its atomic structure, MPc molecules are suitable to Graphite (HOPG) substrate was cleaved in air before being functionalize graphene for chemical sensing. loaded into the vacuum chamber. Afterward, the cleaved The present study employs molecular scale imaging and HOPG sample was annealed at 823 K for 5 h to obtain large, tunneling spectroscopy to investigate NO adsorption on copper ﬂat and clean areas as shown in the STM imaging. phthalocyanine (CuPc) monolayers deposited on highly The CuPc was purchased from Sigma-Aldrich and puriﬁed by oriented pyrolytic graphite (HOPG). The HOPG surface has multiple sublimation cycles. The CuPc monolayer sample was similar electronic properties to graphene, including a nearly deposited as thick overlayers of CuPc on clean Au(111) and inert surface and a zero band gap. NO also was dosed onto HOPG surfaces by organic molecular beam epitaxy with a CuPc/Au(111) for comparison with NO/CuPc/HOPG. Using diﬀerentially pumped eﬀusion cell (Eberl MBE- Komponent- STM, the dependence of NO absorption on the MPc support en), while the sample was in the UHV preparation chamber, as (HOPG vs Au(111)) was elucidated. To understand the shown in Suppoting Information, SI, Figure S1. During electronic changes of the HOPG surface induced by generation deposition, both the Au(111) and HOPG were held at 373 of NO/CuPc/HOPG complexes, DFT calculations were K. Subsequently, the CuPc multilayers on Au(111) were heated performed. to 623 K for 4 min to form a ﬂat-lying monolayer of CuPc on the Au(111) observed by in situ STM, because the CuPc/CuPc ■ EXPERIMENTAL SECTION interactions in multilayers are weaker than the CuPc/Au(111) 33 All experiments were performed in a commercial multichamber surface interaction. Conversely, the CuPc multilayer on Omicron ultrahigh vacuum (UHV) system with a base pressure HOPG was annealed at 473 K for 6 min surface to form a ﬂat- below 1 × 10−10 Torr. Clean Au(111) and HOPG surfaces lying monolayer of CuPc on the HOPG observed by in situ were prepared as substrates for CuPc deposition. The surface of STM. This lower annealing temperature on HOPG results from a single crystal Au(111) was cleaned by multiple sputtering the weaker interaction CuPc with HOPG than with Au(111). cycles with a 0.5 to 1 kV of Ar+ ion beam (RBD instruments) NO was dosed on CuPc monolayer in the UHV chamber at with an Ar background pressure of 6 × 10−5 Torr at 300 K 150 K with use of a pulsed supersonic molecular beam source surface temperature. After sputtering, the Au(111) sample was (General Valve Series 1), which was diﬀerentially pumped using annealed at 773 K for 30 min. This sputtering and annealing a three chamber diﬀerentially pumped source with turbomo- cycle was repeated until an atomically ﬂat Au(111) surface was lecular pumps (TMP). The NO analyte was diluted in He (He:
10077 dx.doi.org/10.1021/jp5002258 | J. Phys. Chem. C 2014, 118, 10076−10082 The Journal of Physical Chemistry C Article
95%; NO: 5%). The low surface temperature was employed so tilting of NO binding consistent with the bound NO that the chemisorbate would be stable on the surface for STM continuously rotating on Cu ion because NO has a single Imaging. The pulsed molecular beam operated at 30 Hz with a bond to Cu. A schematic binding conﬁguration of NO with 100 μs opening time. Note this the supersonic molecular beam CuPc molecules is presented in Figure 1(c). source will produce a nearly monoenergetic beam of NO with Scanning tunneling spectroscopy (STS) was employed to an approximate translational energy of 0.33 eV, so it slightly investigate the changes in the electronic structure of CuPc/ favors direct chemisorption over precursor chemisorption Au(111) and CuPc/HOPG due to NO chemisorption, as compared to a thermal gas source at 300 K.34 Before ﬂowing, shown in Figure 2. It is noted that all dI/dV curves were the diluted NO gas with pulsed valve into preparation chamber, measured on central area of the CuPc molecules, and swept the preparation chamber was pumped only with a turbomo- from −2 to 2 V. During measurement all spectra, STM tips − lecular pump (TMP) and held at 1 × 10 9 Torr. Upon were approached to surface (Δz = ∼0.1 nm) for detecting activating the pulsed NO/He beam, the pressure rose to 2 × larger tunneling signal. Although thick CuPc ﬁlms have a 2.3 eV − 10 7 Torr. The dosing time was 10 min for the data in Figures band gap,36,37 the measured band gaps of CuPc molecules on 1, 2, and 3. After dosing the NO, the samples were transferred Au(111) and HOPG are much smaller; 1.5 eV for NO/CuPc/ Au(111) and 1.75 eV for NO/CuPc/HOPG. The diﬀerence in band gap between these two systems is consistent with the diﬀerence in the density of states (DOS) between Au(111) and HOPG. During STS measurements on CuPc molecules, the STM tips measure tunneling currents not only from CuPc molecules, but also from the Au(111) or HOPG surfaces because the metal tips are within a few angstroms of Au(111) or HOPG.38 Both Au(111) and HOPG have metallic or semimetallic density of states as shown by their zero band gaps in STS, but the Au(111) surface has larger density of states than Figure 3. Empty-state STM images of a CuPc monolayer surface dosed with NO on Au(111) and HOPG. STM images were recorded HOPG. The measured DOS of substrates is mixed with DOS of CuPc, so a narrower band gap appears in STS curves for NO/ with Vs = 2.0 V, It = 20 pA. Scale bars indicate 10 nm. The white circles indicate CuPc molecules with chemisorbed NO. (a) CuPc CuPc/Au(111) than for NO/CuPc/HOPG. monolayer dosed NO for 10 min on Au(111). About 7% of CuPc The STS of the clean CuPc molecules on Au(111) and molecules reacted with NO on CuPc/Au(111). (b) CuPc monolayer HOPG shows the Fermi level (EF, 0 V position in STS) in the dosed NO for 10 min on HOPG. Approximately 0.1% of CuPc middle of the band gap (black curves) shown in Figure 2, both molecules reacted with NO on CuPc/HOPG. The coverage of parts (a) and (b). Unreacted CuPc (black line) has a Fermi saturation NO coverage is much smaller on HOPG than on Au(111). level (EF) almost in the middle of the band gap on both of Au(111) and HOPG. The CuPc monolayer has almost zero immediately to an STM chamber; the sample stage on the STM conductance from −0.5 to 0.5 V, and this zero conductance was maintained at 100 K to minimize analyte desorption. All appears as the band gap. This band gap indicates that unreacted − STM work was performed at <5 × 10 11 Torr, and all STM CuPc molecules act as intrinsic semiconductor in vacuum. images were acquired using electrochemically etched W tips. After NO chemisorption onto CuPc molecules, the Fermi level of CuPc molecules is shifted toward the valence band, ■ RESULTS AND DISCUSSION which corresponds in a molecule to the highest occupied The CuPc monolayer/Au(111) dosed with NO was imaged in molecular orbital (HOMO) of CuPc on both Au(111) and UHV-STM to observe the change induced by NO dosing. All HOPG, as shown in Figure 2. For NO/CuPc chemisorbates on imaging was performed at Vs = 2 V. As shown in an empty state Au(111) surface, the EF shift (blue arrow) is about 0.3 eV STM image of Figure 1, NO chemisorption on a CuPc (Figure 2(a)). This shift of Fermi level is also observed in NO/ monolayer/Au(111) at 150 K results in topographic CuPc/HOPG, as shown in Figure 2(b). After NO chem- modiﬁcation of the Cu atom which is located at the center of isorption on metal center of CuPc, the Fermi level moves about CuPc molecule. The molecular structure of CuPc is clearly 0.25 eV toward the HOMO. However, these NO induced EF deﬁned in a submolecular resolution STM image in Figure 1 shifts on both Au(111) and HOPG might not be denoted as “p- (a). While the outer carbon aromatic rings have 4-fold doping”, but instead are denoted here as dipole-induced shifts symmetry and are bright in STM imaging, the unreacted because the Fermi are still in the band gap on both Au(111) Cu2+ is located in center of the molecule and appears as dark and HOPG. It is noted these shift are consistent with CuPc hole. After chemisorption of NO, the topographic appearance being a net charge donor during reaction with NO on both of core Cu atom is modiﬁed into a bright protrusion, while the substrates. 4-leaf pattern of ring remains. This modiﬁed bright symmetric Although NO chemisorption on CuPc induces Fermi level protrusion, which appears in the center of CuPc, is consistent shifts on both Au(111) and HOPG, the CuPc layers show large with a single NO molecules binding to the Cu atom of CuPc. diﬀerences in saturation NO coverage. After dosing NO from NO chemisorbates are also observed on CuPc/HOPG, as the MBS at 30 Hz with 100 μs opening time for 10 min at 150 shown in Figure 1(b). The topographic appearance of these K, STM images reveals ∼7% of CuPc molecules/Au(111) are chemisorption sites to similar NO/CuPc on Au(111); a dark reacted with NO and form NO chemisorbates in Figure 3(a). hole, which assigned to Cu, is modiﬁed into symmetric bright The dose corresponds to a saturation dose since increasing the spot. It has previously been shown by DFT calculations that dose time twofold did not create more chemisorption sites. It is NO binding with Cu via the N terminal of NO has the highest estimated that the dose corresponds to ∼30 L per each Au stability and the Cu−N−O bond is bent in Figure 1(b).35 atom, since the pressure rise in the chamber was 2 × 10−7 Torr However, STM images do not show observable bending or for 600 s, and a background almost entirely of NO, since the
10078 dx.doi.org/10.1021/jp5002258 | J. Phys. Chem. C 2014, 118, 10076−10082 The Journal of Physical Chemistry C Article
Figure 4. Density Functional Theory models of NO/CuPc/Au(111) and NO/CuPc/graphene. (a) Binding conﬁguration of NO chemisorption site on CuPc/Au(111). (b),(c) Projected density of states of CuPc molecules and Au(111) before and after NO binding on CuPc/Au(111). (d) Binding conﬁguration of NO chemisorption site on CuPc/HOPG. (e),(f) Projected density states of CuPc molecules and graphene before and after NO binding on CuPc/graphene. The NO adsorption induces a decrease of graphene DOS at 1 eV below the Fermi surface (black arrow) in the valence band, while increasing the DOS of CuPc near 4.5 eV below the Fermi surface and 2.5 eV above the Fermi surface in the conduction band (red arrow). The Fermi surface is shifted to zero level on the x-axis in the plots. pressure gauge is insensitive to He and because heavy density of states of the substrate which determines the molecules are concentrated to centerline during expansion in diﬀerence in saturation coverage. the supersonic nozzle of MBS.34 These NO chemisorbates are Density of functional theory calculations were performed to dispersed, i.e., island formation is not observed. After exposing understand the diﬀerences in NO chemisorption and charge NO of equivalent dosage (10 min) on CuPc monolayer transfer for NO/CuPc/Au(111) and NO/CuPc/HOPG, as deposited on HOPG at 150 K, NO dosing also induces shown in Figure 4 and SI Figures S2 and S3 as a complement to saturation coverage of NO on CuPc/HOPG, but the saturation the experiments. The Vienna Ab Initio Simulation Package coverage of NO is much smaller (∼0.1%) on HOPG than on (VASP) was employed to calculate van der Waals corrected − Au(111). Only few CuPc molecules react with NO and form spin-polarized periodic DFT.50 54 For NO on CuPc/Au(111), NO chemisorbates in Figure 3(b). which has binding energy −0.24 eV in Figure 4(a), the density Although NO chemisorbates can be detected on both of states (DOS) of Au(111) shows almost no change upon NO Au(111) and HOPG surfaces, charge transfer behavior is chemisorption even though NO loses electron charge (0.07 e) diﬀerent on each surface. Charge transfer can occur between to CuPc/Au(111). As shown in Figure 4, parts (b) and (c), the CuPc monolayer and substrates. When CuPc molecules initially, Au(111) accepts 0.08 electrons from adsorbate-free monolayers are formed on Au, electron charge is transferred CuPc; after NO chemisorption, Au(111) accepts 0.19 electrons from the CuPc molecules to the Au(111) surface due to band from NO and CuPc. Thus, there is an excess 0.11 electrons − alignment at CuPc/Au(111) interface.39 42 Metal phthalocya- transferred to Au(111) surface. Out of total 0.19 electrons nines have nonuniform charge distribution.43,44 A previous transferred to Au(111) surface, only 0.07 electrons comes from report showed that charge can be transferred from the nitrogen NO (see SI Figure S2) and the remaining 0.12 electrons atoms of CuPc molecules to Au(111) surface via the central Cu transfer from CuPc during NO chemisorption on the surface ion.41 For HOPG, the top layer of HOPG does not have consisted with the Fermi level shift observed in the STS dangling bonds and adsorbates only have weak van der Waals experiments. Due to this electron transfer, the Fermi level of interactions with the π orbitals.45 Therefore, when CuPc CuPc moves toward the valence band (HOMO). Although molecules are deposited on HOPG, the delocalized π electrons negative charge was transferred to the Au(111) surface, there is of CuPc form just a weak π−π van der Waals interaction with nearly negligible change of the Au(111) DOS in Figure 4(b). HOPG. Furthermore, since Evac (vacuum level) of CuPc is Au(111) has a very high density of free electrons; therefore, nearly same with HOPG, very small charge transfer occurs transferred the electrons do not induce noticeable changes in − between CuPc and HOPG.45 49 As shown below in the the Au(111) DOS consistent with a relatively high saturation detailed DFT calculations, these factors are a small eﬀect since coverage for NO/CuPc/Au(111). the binding energy of isolated NO molecule on CuPc is DFT calculation shows NO form chemisorption sites on independent of the substrate; instead, it is the diﬀerence in CuPc/graphene and the DOS of graphene is perturbed by NO
10079 dx.doi.org/10.1021/jp5002258 | J. Phys. Chem. C 2014, 118, 10076−10082 The Journal of Physical Chemistry C Article chemisorption consistent with the low saturated coverage consistent with low saturation coverage. However, even though observed in Figure 3(d). As shown in Figure 4, parts (d)−(f) as the saturation coverage of NO/CuPc/graphene is low, the well as SI Figure S3, the charge transfer is in the opposite electronic structure of graphene can be highly altered, because direction for NO chemisorption on CuPc/graphene and CuPc/ of the very low density of states of graphene. It is noted that Au(111). Initially, HOPG donates 0.025 electrons per CuPc NO adsorption on bare graphene has a very low binding energy molecule to adsorbate-free CuPc; after NO chemisorption, (29 mV) compared to NO/CuPc/HOPG (250 mV).55 HOPG donates an additional 0.025 electrons to both NO and Therefore, it can be expected that chemical sensors based reacted CuPc, and there is a corresponding decrease in the NO/CuPc/graphene will have a few orders of magnitude DOS of graphene at 1 eV below the Fermi surface in the higher sensitivity than that for NO/graphene bare sensors; in valence band. It is noted that DFT calculations show NO general, CuPc and other phthalocyanine functionalization can adsorption on bare graphene has weak binding, 29 mV, and extend the reported sensitivity for bare graphene based sensors induces only small charge transfer (0.018 e); conversely, the of highly reactive molecules (such as NO2) to high sensitivity binding of NO to CuPc/HOPG has stronger binding, 250 mV, for a large range of modestly reactive molecules.8 STM and and induces a charge transfer from HOPG of 0.025 e.55 This DFT results show that functionalization of graphene with MPc means for 300 K sensing the coverage of NO would be many would be a potential candidate for chemical sensing platforms, orders of magnitude greater for CuPc/HOPG than bare HOPG which can be expected to show high chemical sensitivity. thereby increasing the sensor sensitivity. Furthermore, the CuPc/HOPG will be far more selective. Conversely, as shown ■ ASSOCIATED CONTENT in Figure 4(e), NO chemisorption induces an increase of the *S Supporting Information − DOS in CuPc at 4.5 eV. It is noted although CuPc molecules Schematic diagram of STM and MBE chambers, charge density accept electron charge from graphene during NO reaction, diﬀerence plots of NO/CuPc/Au(111), and NO/CuPc/ ∼ CuPc molecules also donates almost all ( 0.05 e) of its excess HOPG. This material is available free of charge via the Internet electrons to NO simultaneously, consistent with Fermi level at http://pubs.acs.org. shift observed in the STS experiments. To conﬁrm the experimental observation of low saturation ■ AUTHOR INFORMATION coverage and the hypothesis of NO chemisorption inducing Corresponding Author signiﬁcant change in the graphene electronic structure, the *Phone: + 01-858-534-3368; e-mail: [email protected] eﬀect of coverage upon NO binding on CuPc/graphene was calculated using a two CuPc molecules/graphene model, as Notes ﬁ shown in Figure 4d and SI Figure S3. The binding energy of The authors declare no competing nancial interest. initial NO chemisorbate on CuPc/HOPG is −0.24 eV, while the neighboring NO chemisorption site has only a −0.12 eV ■ ACKNOWLEDGMENTS binding energy. This decrease of binding energy is consistent This work was supported by NSF Grant CHE-0848502 and by with a decreasing coverage, which results in small saturation STARnet, a Semiconductor Research Corporation program, NO coverage on HOPG. The low DOS of graphene both limits sponsored by MARCO and DARPA and by SRC NRI SWAN. the saturation coverage of NO/CuPc/graphene and likely DFT calculation work was also supported from NSF TeraGrid renders it to be an extremely sensitive chemical sensor. Because (XSEDE) resources under allocation numbers [TG- graphene has a low density of states, even small electronic SEE090006], [TG-DMR110091], and [TG-DMR130127]. perturbations can induce large sensitivity in sensors based on Use of the Center for Nanoscale Materials was supported by graphene.6,7 the US Department of Energy, Oﬃce of Science, Oﬃce of Basic Energy Sciences, under Contract No. DE-AC02-06CH11357. ■ CONCLUSIONS In order to elucidate chemisorption nature of NO with CuPc/ ■ REFERENCES HOPG, scanning tunneling microscopy (STM) was used to (1) Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Zhang, study NO dosed on CuPc monolayers deposited on Au(111) Y.; Dubonos, S. V.; Grigorieva, I. V.; Firsov, A. A. Electric Field Effect − and HOPG. After saturating dosing of NO onto CuPc/ in Atomically Thin Carbon Films. Science 2004, 306, 666 669. Au(111), only, ∼7% of CuPc molecules form chemisorption (2) Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; sites with NO. STS shows that NO induces a Fermi level shift Katsnelson, M. I.; Grigorieva, I. V.; Dubonos, S. V.; Firsov, A. A. Two- Dimensional Gas of Massless Dirac Fermions in Graphene. Nature to from the middle of the band gap toward the valence band 2005, 438, 197−200. (HOMO). After dosing an equal amount of NO on CuPc/ (3) Zhang, Y. B.; Tan, Y. W.; Stormer, H. L.; Kim, P. Experimental HOPG, NO forms only 0.1% chemisorption sites on CuPc/ Observation of the Quantum Hall Effect and Berry’s Phase in HOPG (70× lower than on CuPc/Au(111)), but the Graphene. Nature 2005, 438, 201−204. chemisorption sites and the Fermi level shift appear nearly (4) Fiori, G.; Iannaccone, G. Simulation of Graphene Nanoribbon identical for NO/CuPc/HOPG and NO/CuPc/Au. DFT Field-effect Transistors. IEEE Electron Dev. Lett. 2007, 28, 760−762. calculations show that NO chemisorption with CuPc/ (5) Lemme, M. C.; Echtermeyer, T. J.; Baus, M.; Kurz, H. A − Au(111) induces electron loss for NO and transfer to Graphene Field-Effect Device. IEEE Electron Dev. Lett. 2007, 28, 282 Au(111), but the density of states (DOS) of Au(111) shows 284. negligible change, due to large DOS on Au. Conversely, for (6) Hill, E. W.; Vijayaragahvan, A.; Novoselov, K. Graphene Sensors. IEEE Sens J. 2011, 11, 3161−3170. NO/CuPc/HOPG, negative charge is transferred from (7) He, Q. Y.; Wu, S. X.; Yin, Z. Y.; Zhang, H. Graphene-Based graphene to NO, and there is a large decrease of DOS in Electronic Sensors. Chem. Sci. 2012, 3, 1764−1772. graphene around 1 eV below the Fermi surface in the valence (8) Schedin, F.; Geim, A. K.; Morozov, S. V.; Hill, E. W.; Blake, P.; band. This altered DOS of graphene induces a decreased Katsnelson, M. I.; Novoselov, K. S. Detection of Individual Gas binding energy for NO chemisorption in neighboring sites Molecules Adsorbed on Graphene. Nat. Mater. 2007, 6, 652−655.
10080 dx.doi.org/10.1021/jp5002258 | J. Phys. Chem. C 2014, 118, 10076−10082 The Journal of Physical Chemistry C Article
(9) Dan, Y. P.; Lu, Y.; Kybert, N. J.; Luo, Z. T.; Johnson, A. T. C. (29) Tegeler, E.; Iwan, M.; Koch, E. E. Electronic-Structure of the Intrinsic Response of Graphene Vapor Sensors. Nano Lett. 2009, 9, Valence Bands of H-2-Phthalocyanine, Mg-Phthalocyanine and Pt- 1472−1475. Phthalocyanine Derived from Soft-X-Ray Emission and Photoelectron (10) Joshi, R. K.; Gomez, H.; Alvi, F.; Kumar, A. Graphene Films and Emission-Spectra. J. Electron. Spectrosc. 1981, 22, 297−307. Ribbons for Sensing of O-2, and 100 ppm of CO and NO2 in Practical (30) Martin, M.; Andre, J. J.; Simon, J. Influence of Dioxygen on the Conditions. J. Phys. Chem. C 2010, 114, 6610−6613. Junction Properties of Metallophthalocyanine Based Devices. J. Appl. (11) Schniepp, H. C.; Li, J. L.; McAllister, M. J.; Sai, H.; Herrera- Phys. 1983, 54, 2792−2794. Alonso, M.; Adamson, D. H.; Prud’homme, R. K.; Car, R.; Saville, D. (31) Kerp, H. R.; Westerduin, K. T.; van Veen, A. T.; van Faassen, E. A.; Aksay, I. A. Functionalized Single Graphene Sheets Derived From E. Quantification and Effects of Molecular Oxygen and Water in Zinc Splitting Graphite Oxide. J. Phys. Chem. B 2006, 110, 8535−8539. Phthalocyanine Layers. J. Mater. Res. 2001, 16, 503−511. (12) Stankovich, S.; Dikin, D. A.; Piner, R. D.; Kohlhaas, K. A.; (32) Simon, J.; Andre,́ J. J.; Lehn, J. M.; Rees, C. W. Molecular Kleinhammes, A.; Jia, Y.; Wu, Y.; Nguyen, S. T.; Ruoff, R. S. Synthesis Semiconductors: Photoelectrical Properties and Solar Cells; Springer- of Graphene-Based Nanosheets via Chemical Reduction of Exfoliated Verlag: Berlin/New York, 1985; pp 79−149. Graphite Oxide. Carbon 2007, 45, 1558−1565. (33)Buchholz,J.C.;Somorjai,G.A.Surface-Structuresof (13) Eda, G.; Fanchini, G.; Chhowalla, M. Large-area Ultrathin Films Phthalocyanine Monolayers and Vapor-Grown Films Low-Energy − of Reduced Graphene Oxide as a Transparent and Flexible Electronic Electron-Diffraction Study. J. Chem. Phys. 1977, 66, 573 580. Material. Nat. Nanotechnol. 2008, 3, 270−274. (34) Arumainayagam, C. R.; Madix, R. J. Molecular-Beam Studies of − (14) Fang, Y. X.; Guo, S. J.; Zhu, C. Z.; Zhai, Y. M.; Wang, E. K. Self- Gas-Surface Collision Dynamics. Prog. Surf. Sci. 1991, 38,1 102. Assembly of Cationic Polyelectrolyte-Functionalized Graphene Nano- (35) Nguyen, T. Q.; Escano, M. C. S.; Kasai, H. Nitric Oxide sheets and Gold Nanoparticles: A Two-Dimensional Heterostructure Adsorption Effects on Metal Phthalocyanines. J. Phys. Chem. B 2010, − for Hydrogen Peroxide Sensing. Langmuir 2010, 26, 11277−11282. 114, 10017 10021. (15) Luo, J.; Chen, Y. Z.; Ma, Q.; Liu, R.; Liu, X. Y. Layer-by-Layer (36) Hill, I. G.; Kahn, A.; Soos, Z. G.; Pascal, R. A. Charge-separation Energy in Films of π-Conjugated Organic Molecules. Chem. Phys. Lett. Self-Assembled Hybrid Multilayer Films Based on Poly(sodium 4- − styrenesulfonate) Stabilized Graphene with Polyaniline and their 2000, 327, 181 188. Electrochemical Sensing Properties. RSC Adv. 2013, 3, 17866−17873. (37) Schwieger, T.; Peisert, H.; Golden, M. S.; Knupfer, M.; Fink, J. (16) Wang, Q. H.; Hersam, M. C. Room-temperature Molecular- Electronic Structure of the Organic Semiconductor Copper resolution Characterization of Self-Assembled Organic Monolayers on Phthalocyanine and K-CuPc Studied Using Photoemission Spectros- Epitaxial Graphene. Nat. Chem. 2009, 1, 206−211. copy. Phys. Rev. B 2002, 66. (17) Wright, J. D. Gas-Adsorption on Phthalocyanines and Its Effects (38) Soe, W. H.; Manzano, C.; De Sarkar, A.; Chandrasekhar, N.; on Electrical-Properties. Prog. Surf. Sci. 1989, 31,1−60. Joachim, C. Direct Observation of Molecular Orbitals of Pentacene (18) Archer, P. B. M.; Chadwick, A. V.; Miasik, J. J.; Tamizi, M.; Physisorbed on Au(111) by Scanning Tunneling Microscope. Phys. Rev. Lett. 2009, 102. Wright, J. D. Kinetic Factors in the Response of Organometallic (39) Yan, L.; Watkins, N. J.; Zorba, S.; Gao, Y. L.; Tang, C. W. Semiconductor Gas Sensors. Sens. Actuators 1989, 16, 379−392. Thermodynamic Equilibrium and Metal-Organic Interface Dipole. (19) Ho, K. C.; Tsou, Y. H. Chemiresistor-type NO Gas Sensor Appl. Phys. Lett. 2002, 81, 2752−2754. Based on Nickel Phthalocyanine Thin Films. Sens. Actuators B-Chem. (40) Chen, W.; Wang, L.; Qi, D. C.; Chen, S.; Gao, X. Y.; Wee, A. T. 2001, 77, 253−259. S. Probing the Ultrafast Electron Transfer at the CuPc/Au(111) (20) van Faassen, E.; Kerp, H. Explanation of the Low Oxygen Interface. Appl. Phys. Lett. 2006, 88. Sensitivity of Thin Film Phthalocyanine Gas Sensors. Sens. Actuators B- − (41) Hu, Z. P.; Li, B.; Zhao, A. D.; Yang, J. L.; Hou, J. G. Electronic Chem. 2003, 88, 329 333. and Magnetic Properties of Metal Phthalocyanines on Au(111) (21) Bohrer, F. I.; Colesniuc, C. N.; Park, J.; Ruidiaz, M. E.; Schuller, Surface: A First-Principles Study. J. Phys. Chem. C 2008, 112, 13650− I. K.; Kummel, A. C.; Trogler, W. C. Comparative Gas Sensing in 13655. Cobalt, Nickel, Copper, Zinc, and Metal-Free Phthalocyanine ﬁ − (42) Zhang, Y. Y.; Du, S. X.; Gao, H. J. Binding Con guration, Chemiresistors. J. Am. Chem. Soc. 2009, 131, 478 485. Electronic Structure, and Magnetic Properties of Metal Phthalocya- (22) Grate, J. W.; Klusty, M.; Barger, W. R.; Snow, A. W. Role of nines on a Au(111) Surface Studied with Ab Initio Calculations. Phys. Selective Sorption in Chemiresistor Sensors for Organophosphorus − Rev. B 2011, 84. Detection. Anal. Chem. 1990, 62, 1927 1934. (43) Schaffer, A. M.; Gouterma, M.; Davidson, E. R. Porphyrins 0.28. (23) Ludwig, C.; Strohmaier, R.; Petersen, J.; Gompf, B.; Extended Huckel Calculations on Metal Phthalocyanines and Eisenmenger, W. Epitaxy and Scanning-Tunneling-Microscopy Tetrazaporphins. Theor. Chim. Acta 1973, 30,9−30. Image-Contrast of Copper Phthalocyanine on Graphite and Mos2. J. (44) Figgis, B. N.; Kucharski, E. S.; Reynolds, P. A. Electronic- − Vac Sci. Technol. B 1994, 12, 1963 1966. Structure of Cobalt PhthalocyanineA Charge-Density Study. J. Am. (24) Lu, X.; Hipps, K. W.; Wang, X. D.; Mazur, U. Scanning Chem. Soc. 1989, 111, 1683−1692. Tunneling microscopy of Metal Phthalocyanines: d(7) and d(9) (45) Kera, S.; Yamane, H.; Sakuragi, I.; Okudaira, K. K.; Ueno, N. − Cases. J. Am. Chem. Soc. 1996, 118, 7197 7202. Very Narrow Photoemission Bandwidth of the Highest Occupied State (25) Lu, X.; Hipps, K. W. Scanning Tunneling Microscopy of Metal in a Copper-Phthalocyanine Monolayer. Chem. Phys. Lett. 2002, 364, Phthalocyanines: d(6) and d(8) Cases. J. Phys. Chem. B 1997, 101, 93−98. 5391−5396. (46) Shimada, T.; Hamaguchi, K.; Koma, A.; Ohuchi, F. S. Electronic (26) Nilson, K.; Ahlund, J.; Brena, B.; Gothelid, E.; Schiessling, J.; Structures at the Interfaces between Copper Phthalocyanine and Martensson, N.; Puglia, C. Scanning Tunneling Microscopy Study of Layered Materials. Appl. Phys. Lett. 1998, 72, 1869−1871. Metal-Free Phthalocyanine Monolayer Structures on Graphite. J. (47) Komolov, A. S.; M?ller, P. J. Unoccupied Electronic States and Chem. Phys. 2007, 127. Energy Level Alignment at Interfaces Between Cu-phthalocyanine (27) Wang, Y. F.; Kroger, J.; Berndt, R.; Hofer, W. Structural and Films and Semiconductor Surfaces. Synth. Met. 2003, 138, 119−123. Electronic Properties of Ultrathin Tin-Phthalocyanine Films on (48) Kera, S.; Yabuuchi, Y.; Yamane, H.; Setoyama, H.; Okudaira, K. Ag(111) at the Single-Molecule Level. Angew. Chem., Int. Ed. 2009, K.; Kahn, A.; Ueno, N. Impact of an Interface Dipole Layer on 48, 1261−1265. Molecular Level Alignment at an Organic-Conductor Interface Studied (28) Eley, D. D.; Hazeldin, Dj; Palmer, T. F. Mass-Spectra, by Ultraviolet Photoemission Spectroscopy. Phys. Rev. B 2004, 70. Ionization-Potentials and Related Properties of Metal-Free and (49) Ren, J.; Meng, S.; Wang, Y. L.; Ma, X. C.; Xue, Q. K.; Kaxiras, E. Transition-Metal Phthalocyanines. J. Chem. Soc. Faraday Trans. 2 Properties of Copper (ﬂuoro-)phthalocyanine Layers Deposited on 1973, 69, 1808−1814. Epitaxial Graphene. J. Chem. Phys. 2011, 134.
10081 dx.doi.org/10.1021/jp5002258 | J. Phys. Chem. C 2014, 118, 10076−10082 The Journal of Physical Chemistry C Article
(50) Kresse, G.; Hafner, J. Abinitio Molecular-Dynamics for Liquid- Metals. Phys. Rev. B 1993, 47, 558−561. (51) Kresse, G.; Furthmuller, J. Efficient Iterative Schemes for Ab Initio Total-energy Calculations Using a Alane-wave Basis set. Phys. Rev. B 1996, 54, 11169−11186. (52) Kresse, G.; Furthmuller, J. Efficiency of ab-Initio Total Energy Calculations for Metals and Semiconductors Using a Plane-Wave Basis Set. Comput. Mater. Sci. 1996, 6,15−50. (53) Grimme, S. Semiempirical GGA-Type Density Functional Constructed with a Long-Range Dispersion Correction. J. Comput. Chem. 2006, 27, 1787−1799. (54) Tkatchenko, A.; Scheﬄer, M. Accurate Molecular Van Der Waals Interactions from Ground-State Electron Density and Free- Atom Reference Data. Phys. Rev. Lett. 2009, 102. (55) Leenaerts, O.; Partoens, B.; Peeters, F. M. Adsorption of H(2)O, NH(3), CO, NO(2), and NO on Graphene: A First-Principles Study. Phys. Rev. B 2008, 77.
10082 dx.doi.org/10.1021/jp5002258 | J. Phys. Chem. C 2014, 118, 10076−10082